Understand basic stressstrain response of engineering materials.


 Violet Leonard
 1 years ago
 Views:
Transcription
1 Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities and in particular the fourthorder elasticity or stiffness tensor describing Hooke s Law. Understand the relation between internal material symmetries and macroscopic anisotropy, as well as the implications on the structure of the stiffness tensor. Quantify the response of anisotropic materials to loadings aligned as well as rotated with respect to the material principal axes with emphasis on orthotropic and transverselyisotropic materials. Understand the nature of temperature effects as a source of thermal expansion strains. Quantify the linear elastic stress and strain tensors from experimental straingauge measurements. Quantify the linear elastic stress and strain tensors resulting from special material loading conditions. 3.1 Linear elasticity and Hooke s Law Readings: Reddy BC 2.6 Consider the stress strain curve σ = f(ɛ) of a linear elastic material subjected to uniaxial stress loading conditions (Figure 3.1). 31
2 32 MODUL 3. CONSTITUTIV QUATIONS σ ˆψ = 1 2 ǫ2 1 Figure 3.1: Stressstrain curve for a linear elastic material subject to uniaxial stress σ (Note that this is not uniaxial strain due to Poisson effect) ǫ In this expression, is Young s modulus. Strain nergy Density For a given value of the strain ɛ, the strain energy density (per unit volume) ψ = ˆψ(ɛ), is defined as the area under the curve. In this case, ψ(ɛ) = 1 2 ɛ2 We note, that according to this definition, σ = ˆψ ɛ = ɛ In general, for (possibly nonlinear) elastic materials: σ ij = σ ij (ɛ) = ˆψ ɛ ij (3.1) Generalized Hooke s Law Defines the most general linear relation among all the components of the stress and strain tensor σ ij = C ijkl ɛ kl (3.2) In this expression: C ijkl are the components of the fourthorder stiffness tensor of material properties or lastic moduli. The fourthorder stiffness tensor has 81 and 16 components for threedimensional and twodimensional problems, respectively. The strain energy density in
3 3.2. TRANSFORMATION OF BASIS FOR TH LASTICITY TNSOR COMPONNTS33 this case is a quadratic function of the strain: ˆψ(ɛ) = 1 2 C ijklɛ ij ɛ kl (3.3) Concept Question Derivation of Hooke s law. Derive the Hooke s law from quadratic strain energy function Starting from the quadratic strain energy function and the definition for the stress components given in the notes, 1. derive the Generalized Hooke s law σ ij = C ijkl ɛ kl. 3.2 Transformation of basis for the elasticity tensor components Readings: BC 2.6.2, Reddy The stiffness tensor can be written in two different orthonormal basis as: C = C ijkl e i e j e k e l = C pqrs ẽ p ẽ q ẽ r ẽ s (3.4) As we ve done for first and second order tensors, in order to transform the components from the e i to the ẽ j basis, we take dot products with the basis vectors ẽ j using repeatedly the fact that (e m e n ) ẽ k = (e n ẽ k )e m and obtain: C ijkl = C pqrs (e p ẽ i )(e q ẽ j )(e r ẽ k )(e s ẽ l ) (3.5) 3.3 Symmetries of the stiffness tensor Readings: BC The stiffness tensor has the following minor symmetries which result from the symmetry of the stress and strain tensors: Proof by (generalizable) example: σ ij = σ ji C jikl = C ijkl (3.6) From Hooke s law we have σ 21 = C 21kl ɛ kl, σ 12 = C 12kl ɛ kl and from the symmetry of the stress tensor we have σ 21 = σ 12 Hence C 21kl ɛ kl = C 12kl ɛ kl Also, we have ( C 21kl C 12kl ) ɛkl = 0 Hence C 21kl = C 12kl
4 34 MODUL 3. CONSTITUTIV QUATIONS This reduces the number of material constants from 81 = = In a similar fashion we can make use of the symmetry of the strain tensor ɛ ij = ɛ ji C ijlk = C ijkl (3.7) This further reduces the number of material constants to 36 = 6 6. To further reduce the number of material constants consider equation (10.1), (10.1): σ ij = ˆψ ɛ ij = C ijkl ɛ kl (3.8) 2 ˆψ ɛ mn ɛ ij = C ijkl δ km δ ln = C ijmn = Assuming equivalence of the mixed partials: C ijkl = 2 ˆψ ɛ kl ɛ ij = ( ) Cijkl ɛ kl ɛ mn (3.9) 2 ˆψ ɛ mn ɛ ij (3.10) 2 ˆψ ɛ mn ɛ ij (3.11) 2 ˆψ ɛ ij ɛ kl = C klij (3.12) This further reduces the number of material constants to 21. The most general anisotropic linear elastic material therefore has 21 material constants. We can write the stressstrain relations for a linear elastic material exploiting these symmetries as follows: σ 11 C 1111 C 1122 C 1133 C 1123 C 1113 C 1112 σ 22 C 2222 C 2233 C 2223 C 2213 C 2212 σ 33 σ 23 = C 3333 C 3323 C 3313 C 3312 C 2323 C 2313 C 2312 σ 13 symm C 1313 C 1312 σ 12 C 1212 ɛ 11 ɛ 22 ɛ 33 2ɛ 23 2ɛ 13 2ɛ 12 (3.13) 3.4 ngineering or Voigt notation Since the tensor notation is already lost in the matrix notation, we might as well give indices to all the components that make more sense for matrix operation: σ 1 C 11 C 12 C 13 C 14 C 15 C 16 ɛ 1 σ 2 C 22 C 23 C 24 C 25 C 26 ɛ 2 σ 3 σ 4 = C 33 C 34 C 35 C 36 ɛ 3 C 44 C 45 C 46 ɛ 4 (3.14) σ 5 symm C 55 C 56 ɛ 5 σ 6 C 66 ɛ 6
5 3.5. MATRIAL SYMMTRIS AND ANISOTROPY 35 We have: 1) combined pairs of indices as follows: () 11 () 1, () 22 () 2, () 33 () 3, () 23 () 4, () 13 () 5, () 12 () 6, and, 2) defined the engineering shear strains as the sum of symmetric components, e.g. ɛ 4 = 2ɛ 23 = ɛ 23 + ɛ 32, etc. When the material has symmetries within its structure the number of material constants is reduced even further. We now turn to a brief discussion of material symmetries and anisotropy. 3.5 Material Symmetries and anisotropy Anisotropy refers to the directional dependence of material properties (mechanical or otherwise). It plays an important role in Aerospace Materials due to the wide use of engineered composites. The different types of material anisotropy are determined by the existence of symmetries in the internal structure of the material. The more the internal symmetries, the simpler the structure of the stiffness tensor. ach type of symmetry results in the invariance of the stiffness tensor to a specific symmetry transformations (rotations about specific axes and reflections about specific planes). These symmetry transformations can be represented by an orthogonal second order tensor, i.e. Q = Q ij e i e j, such thatq 1 = Q T and: det(q ij ) = { +1 rotation 1 reflection The invariance of the stiffness tensor under these transformations is expressed as follows: C ijkl = Q ip Q jq Q kr Q ls C pqrs (3.15) Let s take a brief look at various classes of material symmetry, corresponding symmetry transformations, implications on the anisotropy of the material, and the structure of the stiffness tensor: b c y α z γ a β x Triclinic: no symmetry planes, fully anisotropic. α, β, γ < 90 Number of independent coefficients: 21 Symmetry transformation: None C 1111 C 1122 C 1133 C 1123 C 1113 C 1112 C 2222 C 2233 C 2223 C 2213 C 2212 C = C 3333 C 3323 C 3313 C 3312 C 2323 C 2313 C 2312 symm C 1313 C 1312 C 1212
6 36 MODUL 3. CONSTITUTIV QUATIONS b c y α z γ a β x Monoclinic: one symmetry plane (xy). a b c, β = γ = 90, α < 90 Number of independent coefficients: 13 Symmetry transformation: reflection about zaxis Q = C 1111 C 1122 C C 1112 C 2222 C C 2212 C = C C 3312 C 2323 C symm C C 1212 Concept Question Monoclinic symmetry. Let s consider a monoclinic material. 1. Derive the structure of the stiffness tensor for such a material and show that the tensor has 13 independent components. b c y α z γ a β x Orthotropic: three mutually orthogonal planes of reflection symmetry. a b c, α = β = γ = 90 Number of independent coefficients: 9 Symmetry transformations: reflections about all three orthogonal planes Q = Q = Q = C 1111 C 1122 C C 2222 C C = C C symm C C 1212 Concept Question Orthotropic elastic tensor. Consider an orthotropic linear elastic material where 1, 2 and 3 are the orthotropic axes. 1. Use the symmetry transformations corresponding to this material shown in the notes to derive the structure of the elastic tensor. 2. In particular, show that the elastic tensor has 9 independent components.
7 3.5. MATRIAL SYMMTRIS AND ANISOTROPY 37 Concept Question Orthotropic elasticity in plane stress. Let s consider a twodimensional orthotropic material based on the solution of the previous exercise. 1. Determine (in tensor notation) the constitutive relation ε = f(σ) for twodimensional orthotropic material in plane stress as a function of the engineering constants (i.e., Young s modulus, shear modulus and Poisson ratio). 2. Deduce the fourthrank elastic tensor within the constitutive relation σ = f(ε). xpress the components of the stress tensor as a function of the components of both, the elastic tensor and the strain tensor. x z θ y Transversely isotropic: The physical properties are symmetric about an axis that is normal to a plane of isotropy (xyplane in the figure). Three mutually orthogonal planes of reflection symmetry and axial symmetry with respect to zaxis. Number of independent coefficients: 5 Symmetry transformations: reflections about all three orthogonal planes plus all rotations about z axis Q = Q = Q = cos θ sin θ 0 Q = sin θ cos θ 0, 0 θ 2π C 1111 C 1122 C C 1111 C C = C C symm C C 1122 )
8 38 MODUL 3. CONSTITUTIV QUATIONS a a y α γ z a β x Cubic: three mutually orthogonal planes of reflection symmetry plus 90 rotation symmetry with respect to those planes. a = b = c, α = β = γ = 90 Number of independent coefficients: 3 Symmetry transformations: reflections and 90 rotations about all three orthogonal planes Q = Q = Q = Q = Q = Q = C 1111 C 1122 C C 1111 C C = C C symm C C Isotropic linear elastic materials Most general isotropic 4th order isotropic tensor: C ijkl = λδ ij δ kl + µ ( δ ik δ jl + δ il δ jk ) (3.16) Replacing in: σ ij = C ijkl ɛ kl (3.17) gives: σ ij = λδ ij ɛ kk + µ ( ɛ ij + ɛ ji ) (3.18) σ ij = λδ ij ɛ kk + µ ( ɛ ij + ɛ ji ) (3.19) xamples σ 11 = λδ 11 ( ɛ11 + ɛ 22 + ɛ 33 ) + µ ( ɛ11 + ɛ 11 ) = ( λ + 2µ ) ɛ11 + λɛ 22 + λɛ 33 (3.20) σ 12 = 2µɛ 12 (3.21)
9 3.6. ISOTROPIC LINAR LASTIC MATRIALS 39 Concept Question Isotropic linear elastic tensor. Consider an isotropic linear elastic material. 1. Write the threedimensional elastic/stiffness matrix in Voigt notation. Compliance matrix for an isotropic elastic material From experiments one finds: ɛ 11 = 1 [σ 11 ν ( ) ] σ 22 + σ 33 ɛ 22 = 1 [σ 22 ν ( ) ] σ 11 + σ 33 ɛ 33 = 1 [σ 33 ν ( ) ] σ 11 + σ 22 (3.22) 2ɛ 23 = σ 23 G, 2ɛ 13 = σ 13 G, 2ɛ 12 = σ 12 G In these expressions, is the Young s Modulus, ν the Poisson s ratio and G the shear modulus. They are referred to as the engineering constants, since they are obtained from experiments. The shear modulus G is related to the Young s modulus and Poisson ratio ν by the expression G = 2(1+ν). quations (3.22) can be written in the following matrix form: ɛ 11 ɛ 22 ɛ 33 2ɛ 23 2ɛ 13 2ɛ 12 1 ν ν = 1 1 ν (1 + ν) 0 0 symm 2(1 + ν) 0 2(1 + ν) Invert and compare with: σ 11 λ + 2µ λ λ σ 22 λ + 2µ λ σ 33 σ 23 = λ + 2µ µ 0 0 σ 13 symm µ 0 σ 12 µ ɛ 11 ɛ 22 ɛ 33 2ɛ 23 2ɛ 13 2ɛ 12 σ 11 σ 22 σ 33 σ 23 σ 13 σ 12 (3.23) (3.24) and conclude that: λ = ν (1 + ν)(1 2ν), µ = G = 2(1 + ν) (3.25) Concept Question Inverted Hooke s law. Let s consider a linear elastic material.
10 40 MODUL 3. CONSTITUTIV QUATIONS 1. Verify that the compliance form of Hooke s law, quation (3.23) can be written in index notation as: ɛ ij = 1 ] [(1 + ν)σ ij νσ kk δ ij 2. Invert quation (3.23) (e.g. using Mathematica or by hand) and verify quation (3.24) using λ and µ given by (3.25). 3. Verify the expression: σ ij = [ ν ] ɛ ij + (1 + ν) (1 2ν) ɛ kkδ ij Bulk Modulus stablishes a relation between the hydrostatic stress or pressure: p = 1 3 σ kk and the volumetric strain θ = ɛ kk. p = Kθ ; K = 3(1 2ν) (3.26) Concept Question Bulk modulus derivation. Let s consider a linear elastic material. 1. Derive the expression for the bulk modulus in quation (3.26) Concept Question Independent coefficients for linear elastic isotropic materials. For a linearly elastic, homogeneous, isotropic material, the constitutive laws involve three parameters: Young s modulus,, Poisson s ratio, ν, and the shear modulus, G. 1. Write and explain the relation between stress and strain for this kind of material. 2. What is the physical meaning of the coefficients, ν and G? 3. Are these three coefficients independent of each other? If not, derive the expressions that relate them. Indicate also the relationship with the Lame s constants. 4. xplain why the Poisson s ratio is constrained to the range ν ( 1, 1/2). Hint: use the concept of bulk modulus.
11 3.7. THRMOLASTIC FFCTS Thermoelastic effects We are going to consider the strains produced by changes of temperature (ɛ θ ). These strains have inherently a dilatational nature (thermal expansion or contraction) and do not cause any shear. Thermal strains are proportional to temperature changes. For isotropic materials: ɛ θ ij = α θδ ij (3.27) The total strains (ɛ ij ) are then due to the (additive) contribution of the mechanical strains (ɛ M ij ), i.e., those produced by the stresses and the thermal strains: ɛ ij = ɛ M ij + ɛ θ ij σ ij = C ijkl ɛ M kl = C ijkl (ɛ kl ɛ θ kl) or: σ ij = C ijkl (ɛ kl α θδ kl ) (3.28) Concept Question Thermoelastic constitutive equation. Let s consider an isotropic elastic material. 1. Write the relationship between stresses and strains for an isotropic elastic material whose Lamé constants are λ and µ and whose coefficient of thermal expansion is α. Concept Question Thermoelasticity in a fully constrained specimen. Let s consider a specimen which deformations are fully constrained (see Figure 3.2). The material behavior is considered isotropic linear elastic with and ν the elastic constants, the Young s modulus and Poisson s ratio, respectively. A temperature gradient θ is prescribed on the specimen. θ (,ν) Figure 3.2: Specimen fully constrained. 1. Determine the internal stress state within the specimen.
12 42 MODUL 3. CONSTITUTIV QUATIONS Material Mass density [Mg m 3 ] Young s Modulus [GP a] Poisson Ratio Tungsten CFRP Low alloy steels Stainless steel Mild steel Copper Titanium Silicon Silica glass Aluminum alloys GFRP Wood, parallel grain PMMA Polycarbonate Natural Rubbers PVC Thermal xpansion Coefficient [10 6 K 1 Table 3.1: Representative isotropic properties of some materials
13 3.8. PARTICULAR STATS OF STRSS AND STRAIN OF INTRST Particular states of stress and strain of interest Uniaxial stress From (3.23): σ 11 = σ, all stress components vanish ɛ 11 = σ, ɛ 22 = ν σ, ɛ 33 = ν σ, all shear strain components vanish Uniaxial strain ɛ 11 = ɛ, all other strain components vanish From (3.24): σ 11 = (λ + 2µ)ɛ 11 = (1 ν) (1 + ν)(1 2ν) ɛ Plane stress Consider situations in which: σ i3 = 0 (3.29) Then: ɛ 11 = 1 ( ) σ11 νσ 22 (3.30) ɛ 22 = 1 ( ) σ22 νσ 11 (3.31) ɛ 33 = ν ( ) σ11 + σ 22 0!!! (3.32) ɛ 23 = ɛ 13 = 0 (3.33) ɛ 12 = σ 12 2G = (1 + ν)σ 12 (3.34)
14 44 MODUL 3. CONSTITUTIV QUATIONS x2 x3 x1 In matrix form: ɛ 11 ɛ 22 = 1 1 ν 0 σ 11 ν 1 0 σ 22 (3.35) 2ɛ (1 + ν) σ 12 Inverting gives the: Relations among stresses and strains for plane stress: σ 11 σ 22 = σ 12 1 ν 2 1 ν 0 ν (1 ν) 2 ɛ 11 ɛ 22 2ɛ 12 (3.36) Concept Question Plane stress Let s consider an isotropic elastic material for a plate in plane stress state. 1. Determine the outofplane ɛ 33 strain component from the measurement of the inplane normal strains ɛ 11, ɛ Plane strain In this case we consider situations in which: ɛ i3 = 0 (3.37)
15 3.8. PARTICULAR STATS OF STRSS AND STRAIN OF INTRST 45 Then: ɛ 33 = 0 = 1 [ σ 33 ν ( ) ] σ 11 + σ 22, or: (3.38) σ 33 = ν ( ) σ 11 + σ 22 (3.39) ɛ 11 = 1 {σ 11 ν [ σ 22 + ν ( )] } σ 11 + σ 22 = 1 [ (1 ) ν 2 σ 11 ν ( 1 + ν ) ] (3.40) σ 22 ɛ 22 = 1 [ (1 ) ν 2 σ 22 ν ( 1 + ν ) ] σ 11 (3.41) In matrix form: ɛ 11 ɛ 22 = 1 1 ν 2 ν(1 + ν) 0 σ 11 ν(1 + ν) 1 ν 2 0 σ 22 (3.42) 2ɛ (1 + ν) σ 12 Inverting gives the Relations among stresses and strains for plane strain: σ 11 σ 22 = σ 12 (1 + ν)(1 2ν) 1 ν ν 0 ν 1 ν (1 2ν) 2 ɛ 11 ɛ 22 2ɛ 12 (3.43) Concept Question Plane strain. Using Mathematica: 1. Verify equations (3.36) and (3.43) Concept Question Comparison of planestress and planestrain linear isotropic elasticity. Let s consider two linear elastic isotropic materials with the same Young s modulus but different Poisson s ratio, ν = 0 and ν = 1/3. We are interested in comparing the behavior of these two materials for both, plane stress and plane strain models. 1. xpress the relation between the stress components and the strain components in the case of both, plane stress and plane strain models. 2. Under which conditions these two materials manifest the same elastic response for each hypothesis, plane strain and plane stress?
16 46 MODUL 3. CONSTITUTIV QUATIONS 3. Derive the equation that relates ɛ 11 and ɛ 22 when σ 22 = 0 for both, plane strain and plane stress models. For the material having a Poisson s ratio equals to ν = 1/3, for which model (plane stress or plane strain) the deformation ɛ 22 reaches the greatest value? 4. Let s consider a square specimen of each material, with a length equals to 1 m and the origin of the coordinate system is located at the left bottom corner of the specimen. When a deformation of ɛ 11 = 0.01 is applied, calculate the displacement u 2 of the point with coordinates (0.5, 1).
3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationBasic concepts to start Mechanics of Materials
Basic concepts to start Mechanics of Materials Georges Cailletaud Centre des Matériaux Ecole des Mines de Paris/CNRS Notations Notations (maths) (1/2) A vector v (element of a vectorial space) can be seen
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationIn this section, thermoelasticity is considered. By definition, the constitutive relations for Gradθ. This general case
Section.. Thermoelasticity In this section, thermoelasticity is considered. By definition, the constitutive relations for F, θ, Gradθ. This general case such a material depend only on the set of field
More informationEE C247B ME C218 Introduction to MEMS Design Spring 2017
247B/M 28: Introduction to MMS Design Lecture 0m2: Mechanics of Materials CTN 2/6/7 Outline C247B M C28 Introduction to MMS Design Spring 207 Prof. Clark T. Reading: Senturia, Chpt. 8 Lecture Topics:
More informationSolid State Theory Physics 545
olid tate Theory hysics 545 Mechanical properties of materials. Basics. tress and strain. Basic definitions. Normal and hear stresses. Elastic constants. tress tensor. Young modulus. rystal symmetry and
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationConcept Question Comment on the general features of the stressstrain response under this loading condition for both types of materials
Module 5 Material failure Learning Objectives review the basic characteristics of the uniaxial stressstrain curves of ductile and brittle materials understand the need to develop failure criteria for
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationChapter 16: Elastic Solids
Chapter 16: Elastic Solids Chapter 16: Elastic Solids... 366 16.1 Introduction... 367 16.2 The Elastic Strain... 368 16.2.1 The displacement vector... 368 16.2.2 The deformation gradient... 368 16.2.3
More informationPEAT SEISMOLOGY Lecture 9: Anisotropy, attenuation and anelasticity
PEAT8002  SEISMOLOGY Lecture 9: Anisotropy, attenuation and anelasticity Nick Rawlinson Research School of Earth Sciences Australian National University Anisotropy Introduction Most of the theoretical
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam. Isotropic Elastic Models: Invariant vs Principal Formulations
MODELING OF CONCRETE MATERIALS AND STRUCTURES Kaspar Willam University of Colorado at Boulder Class Meeting #2: Nonlinear Elastic Models Isotropic Elastic Models: Invariant vs Principal Formulations Elastic
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More informationCalculating anisotropic physical properties from texture data using the MTEX open source package
Calculating anisotropic physical properties from texture data using the MTEX open source package David Mainprice 1, Ralf Hielscher 2, Helmut Schaeben 3 February 10, 2011 1 Geosciences Montpellier UMR CNRS
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationBasic Concepts of Strain and Tilt. Evelyn Roeloffs, USGS June 2008
Basic Concepts of Strain and Tilt Evelyn Roeloffs, USGS June 2008 1 Coordinates Righthanded coordinate system, with positions along the three axes specified by x,y,z. x,y will usually be horizontal, and
More informationStressinduced transverse isotropy in rocks
Stanford Exploration Project, Report 80, May 15, 2001, pages 1 318 Stressinduced transverse isotropy in rocks Lawrence M. Schwartz, 1 William F. Murphy, III, 1 and James G. Berryman 1 ABSTRACT The application
More informationResource reading (If you would like to brush up on stress, strain, and elasticity):
12.108 Struct. & Prop s. of Earth Mat. Lecture 9 1 Singlecrystal elasticity Assigned Reading: Nye JF (1957) Physical Properties of Crystals. Oxford University Press, Oxford, UK (Chapters 5 and 6). Nye,
More information2 Constitutive Models of Creep
2 Constitutive Models of Creep Analysis of creep in engineering structures requires the formulation and the solution of an initialboundary value problem including the balance equations and the constitutive
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationValidation of the Resonalyser method: an inverse method for material identification
Validation of the Resonalyser method: an inverse method for material identification T. Lauwagie, H. Sol,. Roebben 3, W. Heylen and Y. Shi Katholieke Universiteit Leuven (KUL) Department of Mechanical ngineering
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationProperties of a chiral honeycomb with a Poisson's ratio 1
Properties of a chiral honeycomb with a Poisson's ratio 1 D. Prall, R. S. Lakes Int. J. of Mechanical Sciences, 39, 305314, (1996). Abstract A theoretical and experimental investigation is conducted
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationElements of Rock Mechanics
Elements of Rock Mechanics Stress and strain Creep Constitutive equation Hooke's law Empirical relations Effects of porosity and fluids Anelasticity and viscoelasticity Reading: Shearer, 3 Stress Consider
More informationConstitutive models: Incremental (Hypoelastic) Stress Strain relations. and
Constitutive models: Incremental (Hypoelastic) Stress Strain relations Example 5: an incremental relation based on hyperelasticity strain energy density function and 14.11.2007 1 Constitutive models:
More informationLecture 8 Viscoelasticity and Deformation
HW#5 Due 2/13 (Friday) Lab #1 Due 2/18 (Next Wednesday) For Friday Read: pg 130 168 (rest of Chpt. 4) 1 Poisson s Ratio, μ (pg. 115) Ratio of the strain in the direction perpendicular to the applied force
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More informationTheory of Plasticity. Lecture Notes
Theory of Plasticity Lecture Notes Spring 2012 Contents I Theory of Plasticity 1 1 Mechanical Theory of Plasticity 2 1.1 Field Equations for A Mechanical Theory.................... 2 1.1.1 Straindisplacement
More informationLecture 7. Properties of Materials
MIT 3.00 Fall 2002 c W.C Carter 55 Lecture 7 Properties of Materials Last Time Types of Systems and Types of Processes Division of Total Energy into Kinetic, Potential, and Internal Types of Work: Polarization
More informationSTRESS TRANSPORT MODELLING 2
STRESS TRANSPORT MODELLING 2 T.J. Craft Department of Mechanical, Aerospace & Manufacturing Engineering UMIST, Manchester, UK STRESS TRANSPORT MODELLING 2 p.1 Introduction In the previous lecture we introduced
More informationMathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling
Mathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling Timo Tiihonen & Tero Tuovinen September 11, 2015 European Study Group with Industry, ESGI 112,
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More information2.1 Strain energy functions for incompressible materials
Chapter 2 Strain energy functions The aims of constitutive theories are to develop mathematical models for representing the real behavior of matter, to determine the material response and in general, to
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationBy drawing Mohr s circle, the stress transformation in 2D can be done graphically. + σ x σ y. cos 2θ + τ xy sin 2θ, (1) sin 2θ + τ xy cos 2θ.
Mohr s Circle By drawing Mohr s circle, the stress transformation in D can be done graphically. σ = σ x + σ y τ = σ x σ y + σ x σ y cos θ + τ xy sin θ, 1 sin θ + τ xy cos θ. Note that the angle of rotation,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationTHE GENERAL ELASTICITY PROBLEM IN SOLIDS
Chapter 10 TH GNRAL LASTICITY PROBLM IN SOLIDS In Chapters 35 and 89, we have developed equilibrium, kinematic and constitutive equations for a general threedimensional elastic deformable solid bod.
More informationCIVL4332 L1 Introduction to Finite Element Method
CIVL L Introduction to Finite Element Method CIVL L Introduction to Finite Element Method by Joe Gattas, Faris Albermani Introduction The FEM is a numerical technique for solving physical problems such
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationTransduction Based on Changes in the Energy Stored in an Electrical Field
Lecture 71 Transduction Based on Changes in the Energy Stored in an Electrical Field  Electrostriction The electrostrictive effect is a quadratic dependence of strain or stress on the polarization P
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationLoad Cell Design Using COMSOL Multiphysics
Load Cell Design Using COMSOL Multiphysics Andrei Marchidan, Tarah N. Sullivan and Joseph L. Palladino Department of Engineering, Trinity College, Hartford, CT 06106, USA joseph.palladino@trincoll.edu
More informationCONTINUUM MECHANICS. lecture notes 2003 jp dr.ing. habil. ellen kuhl technical university of kaiserslautern
CONTINUUM MECHANICS lecture notes 2003 jp dr.ing. habil. ellen kuhl technical university of kaiserslautern Contents Tensor calculus. Tensor algebra.................................... Vector algebra.................................
More informationTensor Visualization. CSC 7443: Scientific Information Visualization
Tensor Visualization Tensor data A tensor is a multivariate quantity Scalar is a tensor of rank zero s = s(x,y,z) Vector is a tensor of rank one v = (v x,v y,v z ) For a symmetric tensor of rank 2, its
More informationConstitutive models: Incremental plasticity Drücker s postulate
Constitutive models: Incremental plasticity Drücker s postulate if consistency condition associated plastic law, associated plasticity  plastic flow law associated with the limit (loading) surface Prager
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationANALYSIS OF STRAINS CONCEPT OF STRAIN
ANALYSIS OF STRAINS CONCEPT OF STRAIN Concept of strain : if a bar is subjected to a direct load, and hence a stress the bar will change in length. If the bar has an original length L and changes by an
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationThe Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials under Kinematic Harmonic Loading
Mechanics and Mechanical Engineering Vol. 21, No. 1 (2017) 157 170 c Lodz University of Technology The Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials
More informationTHE MECHANICAL BEHAVIOR OF ORIENTED 3D FIBER STRUCTURES
Lappeenranta University of Technology School of Engineering Science Degree Program in Computational Engineering and Technical Physics Master s Thesis Alla Kliuzheva THE MECHANICAL BEHAVIOR OF ORIENTED
More informationJournal of Basic and Applied Sciences. Australian Journal of Basic and Applied Sciences, 9(37) Special 2015, Pages: ISSN:
ISSN:19918178 Australian Journal of Basic and Applied Sciences Journal home page: www.ajbasweb.com The Development of Unique Orthogonal Rotation Tensor Algorithm in the LLNL DYNA3D for Orthotropic Materials
More informationELECTROMECHANICAL RESPONSE OF PIEZOELECTRIC FOAMS
18 TH INTRNATIONAL CONFRNC ON COMPOSIT MATRIALS LCTROMCHANICAL RSPONS OF PIZOLCTRIC FOAMS K.S. Challagulla 1 *, T.A. Venkatesh 1 School of ngineering, Laurentian University, Sudbury, Canada, Department
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationMAE 323: Chapter 4. Plane Stress and Plane Strain. The Stress Equilibrium Equation
The Stress Equilibrium Equation As we mentioned in Chapter 2, using the Galerkin formulation and a choice of shape functions, we can derive a discretized form of most differential equations. In Structural
More informationBeam Models. Wenbin Yu Utah State University, Logan, Utah April 13, 2012
Beam Models Wenbin Yu Utah State University, Logan, Utah 8434130 April 13, 01 1 Introduction If a structure has one of its dimensions much larger than the other two, such as slender wings, rotor blades,
More information(MPa) compute (a) The traction vector acting on an internal material plane with normal n ( e1 e
EN10: Continuum Mechanics Homework : Kinetics Due 1:00 noon Friday February 4th School of Engineering Brown University 1. For the Cauchy stress tensor with components 100 5 50 0 00 (MPa) compute (a) The
More informationarxiv:condmat/ v1 [condmat.mtrlsci] 10 Jul 2006
Anisotropic properties of mechanical characteristics and auxeticity of cubic crystalline media arxiv:condmat/0607232v1 [condmat.mtrlsci] 10 Jul 2006 T. Paszkiewicz and S. Wolski Chair of Physics, Rzeszów
More information6.37 Determine the modulus of resilience for each of the following alloys:
6.37 Determine the modulus of resilience for each of the following alloys: Yield Strength Material MPa psi Steel alloy 550 80,000 Brass alloy 350 50,750 Aluminum alloy 50 36,50 Titanium alloy 800 116,000
More informationFE FORMULATIONS FOR PLASTICITY
G These slides are designed based on the book: Finite Elements in Plasticity Theory and Practice, D.R.J. Owen and E. Hinton, 1970, Pineridge Press Ltd., Swansea, UK. 1 Course Content: A INTRODUCTION AND
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More informationStress induced seismic velocity anisotropy study Bin Qiu, Mita Sengupta, Jorg Herwanger, WesternGeco/Schlumberger
anisotropy study Bin Qiu, Mita Sengupta, Jorg Herwanger, WesternGeco/Schlumberger Summary A method of calculating stress induced seismic velocity anisotropy is presented and studied. In a first step an
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationENGINEERING COUNCIL CERTIFICATE LEVEL ENGINEERING SCIENCE C103 TUTORIAL 4  STRESS AND STRAIN
NGINRING COUNCIL CRTIFICAT LVL NGINRING SCINC C03 TUTORIAL 4  STRSS AND STRAIN This tutorial ma be skipped if ou are alread familiar with the topic You should judge our progress b completing the self
More information1.1 Stress, strain, and displacement! wave equation
32 geophysics 3: introduction to seismology. Stress, strain, and displacement wave equation From the relationship between stress, strain, and displacement, we can derive a 3D elastic wave equation. Figure.
More informationCHAPTER OBJECTIVES CHAPTER OUTLINE. 4. Axial Load
CHAPTER OBJECTIVES Determine deformation of axially loaded members Develop a method to find support reactions when it cannot be determined from euilibrium euations Analyze the effects of thermal stress
More informationAn acoustic wave equation for orthorhombic anisotropy
Stanford Exploration Project, Report 98, August 1, 1998, pages 6?? An acoustic wave equation for orthorhombic anisotropy Tariq Alkhalifah 1 keywords: Anisotropy, finite difference, modeling ABSTRACT Using
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationChapter 7. Kinematics. 7.1 Tensor fields
Chapter 7 Kinematics 7.1 Tensor fields In fluid mechanics, the fluid flow is described in terms of vector fields or tensor fields such as velocity, stress, pressure, etc. It is important, at the outset,
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationProceedings of the ASME th International Conference on Ocean, Offshore and Arctic Engineering OMAE2016 June 1924, 2016, Busan, South Korea
Proceedings of the ASME 26 35th International Conference on Ocean, Offshore and Arctic Engineering OMAE26 June 924, 26, Busan, South Korea OMAE2654554 LOCAL STRAIN AND STRESS CALCULATION METHODS OF IRREGULAR
More informationSymmetric Bending of Beams
Symmetric Bending of Beams beam is any long structural member on which loads act perpendicular to the longitudinal axis. Learning objectives Understand the theory, its limitations and its applications
More informationPEAT SEISMOLOGY Lecture 3: The elastic wave equation
PEAT8002  SEISMOLOGY Lecture 3: The elastic wave equation Nick Rawlinson Research School of Earth Sciences Australian National University Equation of motion The equation of motion can be derived by considering
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationproperties Michele Catti Dipartimento di Scienza dei Materiali Università di Milano Bicocca, Italy
Elastic and piezoelectric tensorial properties Michele Catti Dipartimento di Scienza dei Materiali Università di Milano Bicocca, Italy (catti@mater.unimib.it) 1 Tensorial physical properties of crystals
More informationENGN 2290: Plasticity Computational plasticity in Abaqus
ENGN 229: Plasticity Computational plasticity in Abaqus The purpose of these exercises is to build a familiarity with using usermaterial subroutines (UMATs) in Abaqus/Standard. Abaqus/Standard is a finiteelement
More information